1 reactive printing
Primary dyeing (including semi-bleaching or bleaching, but not fixed and soft dyeing vat)dry cloth (color cloth 150, bleached cloth 130) CROSS-FINISHING section for P.S (super-water setting, color cloth 160, bleached cloth 150) printing (reactive pulp, circular screen or flat machine printing, 130 65 Depending on the color depth and fastness to fix the color) dry cloth (color cloth 150, bleached cloth 130) finished product finalization (soft oil or resin) product inspection cloth (plugging, movement, etc.).
2 pigment printing
Dyeing or bleaching (including semi-bleaching or bleaching, but not fixed and soft dyeing vat) Dry cloth (color cloth 150, bleached cloth 130) Intersection finishing for P.S (super-water setting, color cloth 160, bleached cloth 150) Printing (pigment pulp base, screen or flat machine printing, 150 Intersection finishing for dry setting (depending on printing area or fastness) Finished product setting Type (soft oil or resin) to check cloth (plug net, walk, etc.).
3 paste printing
Dyeing base color (non-fixable and soft dyeing vat) dry cloth (150 C) finishing department to do P.S (over-water setting, 160 C) printing (pulp base, circular screen or flat machine printing, 150 C dry cloth) dry finishing section (color drawing 170 C X24m / min dry setting, white drawing 160 C X24m / min dry setting) dyeing Department washing water (washing cold water, cylinder color fixing) dry cloth (150 dry setting). The product is finalized (soft oil or resin) to check cloth (plug net, walk, etc.).
Pigment printing is suitable for all kinds of fiber fabrics. Knitted fabrics have a soft handle and are easily deformed by tension. Therefore, it is required that the adhesive used should have a good handle and easy conjunctiva.
It can be used in Accra Ming F adhesive, adhesive BH, 707 or some other low temperature adhesives.
Coatings/g x urea/g 50 water/g y adhesive/g 400~500 emulsion paste A/g 200 crosslinking agent FH/g 15~25 total amount/g 1000
Printing, drying and fixing. The fixing process enables the crosslinking agent and the crosslinking agent to fully crosslink, improve the fastness and further volatilize the kerosene. Fixation can be done by hanging steam, at 100 C, 57min, or baking, 120~130 C, 1.5 ~ 2min. When printing, the crosslinking agent should be added less and later so as not to affect the feel of printing and fabric. In addition, the emulsion paste or water should be diluted first, and then added to the adhesive pastes to prevent local crosslinking of the colorants.